### Design of Photonic Crystals by FDTD Method *and Fabrication of High-Q Three-Dimensional *

### Photonic Crystal Nanocavities

(有限差分時間領域法によるフォトニック結晶の設計と
高*Q 値 3 次元フォトニック結晶ナノ共振器の作製に関する研究) *

A Dissertation

Submitted to the Graduate School of the University of Tokyo

in Partial Fulfillment of the Requirements for the Degree of

Doctor of Philosophy

タンデーシーヌラット アニワット Tandaechanurat Aniwat

### December 2008

*To my family and my wife *

**Acknowledgement **

First of all I would like to express my deep and sincere gratitude to my supervisor, Professor Yasuhiko Arakawa for giving me a great opportunity to join this laboratory and agreeing to supervise this thesis. His knowledge, experience, and vision have stimulated my enthusiasm for pushing the forefront of research. Without his guidance and mentorship, this work would not have come to fruition.

I would like to thank Professor Yoshiaki Nakano, Professor Kazuhiko Hirakawa, Professor Masaaki Tanaka, Professor Takuji Takahashi, and Professor Satoshi Iwamoto for their useful comments and advices as members of the thesis defense committee.

In particular I would like to thank Professor Satoshi Iwamoto for all of his support and important guidance. Working with him from pretty much the beginning of this work has shaped my path toward a university career, and I want to thank him for that. His editing on papers and ideas expressed there were always the best check.

His wide knowledge and his logical way of thinking have been of great value for me.

I would like to thank the former and current members of the Professor Arakawa group for their input and companionship on this long journey. Their intelligence, dedication, and fantastic personalities have made it a great learning experience. First of all, I wish to express my warm and sincere thanks to Professor Masatoshi Kitamura and Professor Toshihiro Nakaoka for their advices and supports.

I have had great luck to work with some very talented and motivated people on research. In particular, I want to thank my close collaborators on the three- dimensional photonic crystal project, Satomi Ishida – it has been really great working with him. Many great suggestions and different perspectives of him on our collaboration works have enlightened me a lot. Also, I would like to thank Professor Denis Guimard for his tireless effort on growth of samples. His quantum dots are always in best quality. I greatly thank Dr. Kanna Aoki for her pioneer work in

dimensional structures. I learned a lot working with Dr. Masahiro Nomura in the fabrication processes and optical measurements and want to thank him for the consistent positive attitude and all the help.

Also, I would like to thank Mr. Masao Nishioka, Dr. Katsuyuki Watanabe, Dr. Naoto Kumagai, Dr. Damien Bordel for the growth of epitaxy wafer. I also want to acknowledge all of my colleagues and friends in the group: Dr. Toshio Saito, Dr.

Satoshi Kako, Dr. Munetaka Arita, Mr. Toshiyuki Miyazawa, Dr. Tetsuo Kodera, Dr.

Katsuaki Tanabe, Dr. Jong Ho Na, Mr. Christian Kindel, Mr. Takeshi Kawano, Mr.

Mohan Rajesh, Mr. Yuki Wakayama, Mr. Hiroaki Oishi, Mr. Yasutomo Ota, Mr.

Kenichi Ohno, Mr. Shigeru Nakayama, Mr. Kazumasa Miyagawa, Ms. Ayako Suzuki, Mr. Satoru Nakagawa, Mr. Ryo Morihara, Mr. Kihyun Choi, Mr. Woogun Kang, and Mr. Naoya Shinomori. It has been great working and hanging out with them. I would like to thank our group’s secretary: Ms. Mio Ono, Ms. Keiko Okumura, Ms. Masako Ogawa, and Ms. Chieko Sasakawa. Their kindness and supports help me do research smoothly.

I would like to acknowledge financial support from Special Coordination Funds for Promoting Science and technology.

On more personal grounds, my special gratitude is due to my family: dad, mom, Yui, and Lek. Without them, life would be an aimless wander without direction.

They have served as a basis for everything I do and everything I am today.

Last and most importantly of all, I owe my loving thanks to my wife, Pim, for being with me at all the good and bad time. I could not have finished this thesis without my wife’s support. She always gives me joyful home environments and makes me smile every single day. I would like to dedicate this thesis to her.

**Abstract **

Photonic crystal with a defect as a nanocavity has been attracting much
interest as a promising platform to manipulate light and light-matter interaction on
wavelength-sized length scale due to existence of photonic bandgap. The Finite-
Difference Time-Domain (FDTD) method has been widely exploited as a powerful
tool to simulate Maxwell’s equations in photonic crystal structures, enabling ones to
*design novel devices. After two decades of intense development, performance of two-*
*dimensional photonic crystal cavities, in term of quality (Q) factor, has reached *
*saturation, in which experimental Q factors exceed a million with mode volume in the *
order of cubic wavelengths. However, there are still two issues needed to be
*considered. The first one is that those high Q cavities are usually sensitive to change *
in the cavity geometry inflicted by fabrication imperfections. The other one is their
flexibility in applications. Generally, they can only be applied to material systems
with sufficiently high index-contrast and with proper polarization, in which a photonic
*bandgap exists. On the other hand, progress in three-dimensional photonic crystal *
cavities is far behind that in two-dimensional system due to the difficulty in
fabrication, in which a number of photonic crystal periods surrounding the cavity that
can be fabricated is limited. This suggests that, considering current fabrication
*technologies, designs of high Q cavities that can be achieved even with small *
structural size, which is practical in fabrication, are required in order to demonstrate
*high Q cavities. This thesis aims to fill in the abovementioned gaps. Original research *
*work on designs and fabrications of high Q nanocavities in both two- and three-*
dimensional photonic crystals are presented.

In Chapter 2, basic principles of photonic crystals that are necessary for understanding the research background and motivation of this thesis are introduced.

Two-dimensional photonic crystal slabs with both triangular and square lattices and three-dimensional woodpile photonic crystal structures are described in details as they

geometry and structural parameters on the behavior of characteristics of photonic crystals, such as photonic bandgap, resonant frequencies, is discussed. Finally, defects are introduced by adding dielectric materials to perfect crystals to form nanocavities.

In Chapter 3, details on computational methods used in this thesis, which are all based on the FDTD method, are described. The FDTD simulations are categorized into two classes with different boundary conditions, depending on the types of calculations to obtain efficient and accurate solution of electromagnetic waves. The applications of the 3D FDTD calculations to investigate photonic band structures, equi-frequency contours, resonant frequencies, field distributions, quality factors, mode volumes, and effective refractive indices are shown.

*In Chapter 4, a significant increase of Q-factor of dipole modes in photonic *
crystal H1-defect nanocavity after closing of the photonic bandgap are numerically
and experimentally demonstrated by optimizing the slab thickness. The optimal slab
thickness is equal to a wavelength of light confined in the cavity. The strong light
confinement of the cavity in the in-plane direction is not caused by the photonic
bandgap effect due to a lack of the photonic bandgap but resulted from the decoupling
between the cavity mode and the guided mode in the momentum space. Because the
slab thickness, which is the design parameter, can be precisely controlled by using
epitaxial growth techniques, the parameter of the best fabricated cavity and that of the
predicted one are almost exactly the same. This finding will contribute to extending
the freedom of cavity design, such as that for the application to polarization entangled
*photon source, where it is required to form cavity modes with prescribed Q factor and *
polarization.

*In Chapter 5, a photonic crystal nanocavity with an ultra-high Q and small *
mode volume even there is no bandgap is presented. The air hole radii are modulated
with a quadratic profile to decouple the cavity mode from possible losses consisting
of guiding loss and radiation loss, resulting in doubly-degenerated modes with a ratio
*of Q to mode volume of two times higher than the highest value reported so far for *
doubly-degenerated modes. Therefore, this cavity is very promising for the realization
of entangled photon sources. The designed cavity is also shown to be successfully
*applied to achieve high Q cavities for material with low index and for quantum cascade *
lasers, in which a lack of photonic bandgap usually hinders them from applications.

photonic crystal cavities to improve their performances, while the photonic bandgap is
*no longer a preliminary requirement to achieve high Q. *

*In Chapter 6, three designs of high-Q cavities in three-dimensional photonic *
crystals with finite structural size that can be practically fabricated are presented.

*High-Q cavity modes in square-shaped and rectangular-shaped nanocavities are *
achieved by tuning their frequencies to midgap frequency of a complete photonic
bandgap, where light confinement is strongest, by means of optimizing size of the
defects to gain an advantage from the photonic bandgap effect as much as possible.

*Apart from tuning cavity modes to the midgap frequency, the Q factor can be further *
improved by modifying cavity structure through shifting of dielectric rods
*surrounding the cavity. 4.3-time improvement of Q compared with the structure *
without modification of the cavity structure is obtained with a value of 73,300.

*Importantly, this high Q cavity only needs 17 stacked layers to obtain such high Q. *

*These designed cavities show a great promise in the realization of high Q cavities *
using current fabrication technologies.

*In Chapter 7, experimental demonstrations of two high-Q cavities coupled *
with quantum dots in three-dimensional photonic crystals fabricated by using
micromanipulation techniques are presented. The structures are shown to have very
small stacking errors in order of 50 nm, in spite of their large number of the stacked
layers. The square-shaped defect cavity in a 25-layer woodpile layer exhibits a cavity
*mode with Q factor of more than 8,600, which is the highest Q among those for three-*
*dimensional photonic crystal cavities reported so far. The high-Q nature of the cavity *
has been confirmed to be originated not only from a large number of the stacked
layers, but also from the strong localization of the cavity mode when it was tuned to
*the midgap frequency of the complete photonic bandgap. The obtained cavity-Q can *
still be improved to more than 10,000 by finer tuning the cavity mode to the exact
*midgap. For the rectangular-shaped cavity, a cavity mode with Q factor of more than *
*7,700 is obtained by choosing a cavity mode with high theoretical Q and tuning it to *
the midgap. The cavity mode has mode volume as small as 2 cubic half-wavelengths,
*approaching the diffraction limit value. These high Q/V**eff* cavities will give three-
dimensional photonic crystals a wide-open opportunity for the realization of the
applications concerning the full control of light-matter interaction and an ultra-small
optical three-dimensionally-integrated circuit.

In Chapter 8, conclusions to this thesis are presented. Implications of the results presented in this thesis are discussed. The outlook for future research and development is also given.

One may expect it to take quite some time for an ultra-small optical three- dimensionally-integrated circuit based on photonic crystals to be realized and implemented. Nevertheless, the results obtained in this thesis provide one important step towards the acquisition of complete manipulation of light.

**Contents **

**Acknowledgements **** ** i

**Abstract**** **** **** **iii

**1 ** **Introduction **** **** 1 **

1.1 Research background** **1

1.2 Thesis objectives 5

1.3 Thesis outline 6

**2 ** **Basis for Theoretical Analysis of Photonic Crystal**** **11

2.1 Maxwell’s equations and the Bloch-Floquet theorem 11

2.2 Origin of photonic bandgap 14

2.3 Types of photonic crystal 17

2.4 Two-dimensional photonic crystal slabs 18

2.4.1 Comparison between square and triangular photonic crystal lattices 21

2.4.2 Effect of slab thickness and radius of air holes on photonic bandgap 23

2.5 Woodpile structures^{ } 27

2.6 Photonic crystal defect nanocavities^{ } ^{ }29

2.7 Summary^{ } ^{ }33

**3 ** **Finite-Difference Time-Domain Method**^{ }** ^{ }**35

3.1 The Yee algorithm^{ } ^{ }35

3.2 Boundary conditions^{ } ^{ }38

3.2.1 Absorbing boundary condition^{ } ^{ }38

3.2.2 Periodic boundary condition^{ } ^{ } ^{ }42

3.3 FDTD-simulations of photonic crystals^{ } ^{ }44

3.3.1 Band structures and equi-frequency contours^{ } ^{ }44

3.3.2 Cavity characteristics^{ } ^{ }45

3.4 Summary^{ } 51

**4 ** **High-Q Photonic Crystal Nanocavity after Closing of Photonic ****Bandgap with Optimal Slab Thickness**^{ } ^{ }53

4.1 Introduction^{ } ^{ }53

4.2 Structural parameters and defect modes^{ } ^{ }54

*4.3 Increase of cavity Q of H1 dipole modes by optimizing slab thickness*^{ } ^{ }58

4.4 Fabrication Processes^{ } ^{ } ^{ }67

4.5 Optical characterization^{ } ^{ }71

4.5.1 Experimental setup of photoluminescence measurements^{ } ^{ }71

4.5.2 Experimental results^{ } ^{ } ^{ }71

4.6 Summary^{ } ^{ }78

**5 ** **High-Q Photonic Crystal Nanocavity without Photonic Bandgap by ****Modulating Air Hole Radii in Square Lattice**^{ } ^{ } ^{ }79

5.1 Introduction^{ } ^{ }79

5.2 Cavity structures and defect modes^{ } ^{ }80

*5.3 High cavity Q in graded photonic crystal structure by mode decoupling*^{ } ^{ }85

5.3.1 Graded photonic crystal nanocavity with modulating air hole
radii^{ } ^{ }85

*5.3.2 Improvement of cavity Q in graded structure by mode *
decoupling^{ } ^{ }87

*5.4 Applications of high-Q graded photonic crystal cavities*^{ } ^{ }96

*5.4.1 High-Q graded photonic crystal nanocavity with low refractive *
index^{ } ^{ } ^{ }96

5.4.2 Reduction of threshold current of quantum cascade lasers by
graded photonic crystal cavity^{ } ^{ }98

5.4.3 Prospects of graded photonic crystal nanocavity for highly
efficient entangled photon sources^{ } 100

5.5 Summary^{ } 101
**6 ** **Designs of High-Q Nanocavities in Three-Dimensional Photonic **

6.1 Introduction^{ } 103
*6.2 Designs of high-Q nanocavities in woodpile photonic crystals by tuning *

cavity modes to photonic midgap^{ } 105

6.2.1 Square-shaped defect nanocavity^{ } ^{ } 105
6.2.2 Rectangular-shaped defect nanocavity^{ } 113
*6.3 Further improvement of cavity Q by shifting rods in cavity *

neighborhood^{ } 118

6.3.1 Structural parameters and cavity mode^{ } 119
*6.3.2 Enhancing Q factor by fine shifting dielectric rods*^{ } 121
6.3.3 Comparison with double-heterostructure three-dimensional

photonic crystal nanocavity^{ } 125

6.4 Summary^{ } 127

**7 ** **Fabrication and Characterization of High-Q Three-Dimensional **

**Photonic Crystal Nanocavities**^{ } 129

7.1 Introduction^{ } 129

7.2 Fabrication of three-dimensional photonic crystal nanocavities by

micromanipulation techniques^{ } 131

7.2.1 Principles of micromanipulation techniques^{ } 131
7.2.2 Preparations of micromanipulation components and samples 133

7.2.2.1 Probe and posts^{ } 133

7.2.2.2 Plates^{ } 136

7.2.3 Assembly into three-dimensional structures by

micromanipulation^{ } 141

7.3 Experimental setup of photoluminescence measurements^{ } 144
7.4 Results of photoluminescence measurements^{ } 145

7.4.1 Square-shaped defect nanocavity^{ } 145

7.4.2 Rectangular-shaped defect nanocavity^{ } 149

7.5 Summary^{ } 153

**8 ** **Conclusions and Future Outlook**^{ } 155

8.1 Conclusions^{ } 155

8.2 Future Outlook^{ } 158

**References**^{ } 159

**List of Publications**^{ } 169

**Chapter 1 ** **Introduction **

**1.1 Research background **

Photonic crystals are periodic structures made of dielectric materials.

Regions with different dielectric constants alternate periodically and the period is of the order of the wavelength of light. Then, as light propagates inside the periodic material, it reflects at each interface of the different dielectric materials, in the same way as electron experiencing a periodic potential in a semiconductor crystal [1]. As a result of interference, total reflection occurs at specific wavelength-period combinations. Light with this specific wavelength cannot propagate or exist inside the photonic crystal. These forbidden wavelengths or frequencies form a bandgap for light, which is the basis of operation of photonic crystals, in analogy with forbidden energy bands in electronic system. This phenomenon is also present in the nature, for example, the wings of certain butterflies and moths are covered with periodic microscopic structures, which act as photonic crystals [2-4]. The wings reflect light that has a wavelength in the bandgap of the photonic crystal. This effect is seen as the color of the wings. Classes of photonic crystals are distinguished depending on the dimensionality of spatial periodicity. While the one-dimensional structures have been adopted for various lasers for more than three decades such as distributed feedback laser diodes [5-7] and vertical cavity surface-emitting lasers (VCSELs) [8,9], the extension of photonic crystals to two and three dimensions was simultaneously proposed by Yablonovitch and John in 1987 [10,11]. The first one dealt with the possibility of inhabiting spontaneous emission of electromagnetic radiation using three-dimensionally periodic structure. The latter paper discussed the strong localization of photons in defect intentionally introduced into the perfect lattice, resulting in trapping of electromagnetic radiation in the forbidden gap. Their works

have stimulated attention of researchers from all over the world in these new prospects in photonics. In the first decade after the proposal, most of work on photonic crystals has been concentrated on efforts to realize structures with a complete photonic bandgap, in which light is prohibited to propagate in all three directions. Such structures, of course, needs to be periodic in three dimensions. Three criteria were considered to seek for the structure and material that were capable to open the gap. A lattice with a first Brillouin zone closest to a spherical shape would help since gap for different directions would appear at similar energies. The best lattice for a photonic bandgap is thus the triangular lattice in two-dimensional structure and the face-centered-cubic in three-dimensional structure. In addition, an asymmetry lattice was necessary to break the degeneracy of the three-dimensional photonic band and open the gap [12]. As a consequence, most of all the three- dimensional photonic bandgap structures realized up to now are based on the diamond structure [12,13]., an fcc structure with two optical atoms per unit cell. And in order to achieve an overlapping of the gaps at every point of the Brillouin zone boundary, a high refractive index contrast between the composing materials was required [10].

The first experimental demonstration of complete-photonic-bandgap materials
appeared in 1991, which was based on a face-center-cubic (fcc) lattice, presented by
*Yablonovitch et al. [13,14]. The structural size was in centimeter order for the *
microwave regime. Since then many efforts have been concentrated to scale the
various three-dimensional structures down to the visible or near-infrared regime [15-
20]. In application points of view, three-dimensional photonic crystals have been
something disappointing, in spite of their ideal capability to fully control the light.

One of the most promising goals of photonic crystals is an ultra-small optical three-
dimensionally-integrated circuit [21], which combines ultra-low threshold lasers
arrays, sharp bend waveguides, an optical modulator, wavelength selectors, and so on,
*on one optical chip. However, only sharp bend waveguides in line-defect-embedded *
three-dimensional photonic crystals with low losses have been implemented so far
[18,22-24]. Although three-dimensional photonic crystals offer a promise to realize an
efficient nanocavity, by introducing a three-dimensionally-localized defect into a
perfect crystal, because light can be strongly confined in very small volume for a long
*period of time due to Bragg reflection in all three directions, quality (Q) factors of *

crystals. Especially when a light-emitting element and an artificial defect cavity are to
be introduced into the three-dimensional structure to generate a light-emitting device,
a fabrication technique that can simultaneously fulfil requirements of introduction of
an artificial defect and a light-emitting element into the three-dimensional structure is
essential. The existing techniques, such as colloidal self-assembly [25-31], direct
writing by two-photon polymerization [32-35], and multibeam interference
lithography [36-39], can carry out each of the requirement, but not both at the same
time. Layer-by-layer method [15-17,40] and wafer-fusion method [18,19,41,42] have
been shown to have a capability to accomplish the task. Nevertheless, their
complicated procedures together with damage inflicted on the fine structure by
multiple etching and heat treatment preclude them from making three-dimensional
structures with large number of periods and with good quality, leading to a cavity
*with low Q factor of no more than several hundreds [40,43,44]. In contrast, *
micromanipulation techniques do not undergo such problem [45,46]. All photonic
crystal components used to construct three-dimensional structure can be prepared
using a single semiconductor processing sequence and no heating, enables
components to be assembled with high precision and minimum damage to their fine
structure irrespective of materials or complexity of photonic patterns. Therefore,
micromanipulation technique is capable of introducing a defect cavity and light-
emitting elements into the structure at arbitrary positions. Recently, a cavity in
*woodpile structure with a record-Q of 2,300 has been reported with 17 stacked layers *
*using micromanipulation techniques [47]. Yet, this Q seems to be insufficient to *
*pursue ultimate applications, such as thresholdless lasers [48]. High-Q cavity in three-*
dimensional photonic crystals still poses a great challenge to be realized. The low
*value of Q is partly resulted from the restricted structural size of photonic crystals that *
can be fabricated. There are two approaches, which should be done in parallel, to
*enhance the Q. One is the development of the fabrication techniques, which allow a *
larger size of photonic crystals to be made. The other one is to improve the cavity
*designs to be able to have high Q even with a limited size. If such a cavity can be *
achieved, not only the ultimate lasers, but also an ideal semiconductor system for
*demonstrating genuine strong coupling between three-dimensionally confined photon *
and electron may be obtained by introducing a single quantum dot [49] into the cavity
[50,51].

Fabrication of three-dimensional photonic crystal structures is still a difficult process, and a more appealing approach is based on the use of lower-dimensional photonic crystals. Therefore, many of researchers have turned their attention to two- dimensional photonic crystals, whose periodicity is in two dimensions [52-56].

However, because such structures must be infinitely long in the direction
perpendicular to the plane in which two-dimensional periodicity exists, they are not
practical for applications since only finite height structures can be fabricated. A
structure that have been attracted a lot of attention is a finite-thick semiconductor slab
perforated with a two-dimensional lattice of holes [57-62]. Then, the two-dimensional
photonic crystal slab can be easily fabricated following the standard microlithographic
techniques and still retain most of the important features of full three-dimensional
photonic crystals. In photonic crystal slabs, the localization of light in the vertical
direction is controlled by the total internal reflection resulting from the high index
contrast between the high-index slab and the low-index environment. On the other
hand, the confinement in the in-plane direction is controlled by the Bragg reflection
resulting from the photonic crystal lattice. Light in the photonic crystal slab cavity
that does not fulfill the condition for the total internal reflection radiates vertically out
*of the cavity and thus limits Q factor of the cavity, while losses into the in-plane *
direction can be reduced exponentially with the number of photonic crystal layers
surrounding the cavity. In 1999, when first photonic crystal defect cavity lasers was
*demonstrated, a Q of around 250 was reported for a single point defect [63]. Since *
*then there have been various attempts to improve the Q factor. Thanks to the excellent *
suitability of the Finite-Difference Time-Domain (FDTD) method [64] to simulate
light field dynamics and propagation in photonic crystal strctures and the flexibility in
the design of two-dimensional photonic crystal slab nanocavities, various designs of
*ultra-high Q nanocavities have already been succeeded by, such as fine tuning of *
shape, size, and position of air holes near the cavity site [65-71] and exploiting a
*photonic crystal waveguide mode confined in a mode gap [72,73]. Designed Qs in the *
order of 10^{7}-10^{8} has been achieved [72,73]. With the maturation of nanometer-size
photonic crystal fabrication technology in past ten years, photonic crystal nanocavities
*with a passive Q factor of more than one million have been experimentally *
demonstrated [74,75]. However, most of designs of those structures are based on the

*of the cavity geometry in practical fabrication to achieve high Qs. Small variations in *
*the geometry could easily reduce the Q by a factor of 10 [76]. This lack of robustness *
to changes in the cavity geometry becomes a great difficulty to practically fabricate
the device with quality as good as the simulation results.

Photonic bandgap has been shown above to be a great implement for
*confining light. There is a restrict rule of thumb in design of high-Q photonic crystal *
cavities, in which cavity modes must be properly designed to fall in the photonic
bandgap to assure the strong light confinement in the in-plane direction, otherwise
the light mode could couple with guided modes and leak out of the cavity. However,
in some material systems, such as low-index materials [77-79] and quantum cascade
lasers [80-82], which also desire to couple with localized optical modes in photonic
*crystal cavities with high Q to improve their performances, the photonic bandgap *
does not exist in a frequency range of interest, i.e., the photonic bandgap for the
structure with low refractive index only exists in very high frequency range, while
there is no photonic bandgap for light polarized in transverse magnetic (TM) -like
mode, where photons are polarized in quantum cascade lasers, in the photonic crystal
slab with air holes [60]. Search for cavity designs suitable for these material systems
is still ongoing.

**1.2 Thesis objectives **

After more than two decades since the proposal of photonic crystals, the
*performance of two-dimensional photonic crystal slab cavities, in term of cavity-Q, *
*has reached saturation, in which experimental Q factors exceed a million with mode *
volume in the order of cubic wavelengths. It is thus interesting to divert the
development of cavity designs to robustness of cavities to fabrication imperfections,
which usually degrade the cavity performance from the design. In addition, a
*predesignated condition, in which a photonic bandgap is essential to achieve high Q, *
should be compromised to extend the scope of optical devices that can utilize
photonic crystal cavities to improve their performance. Compared to the two-
dimensional system, progress in three-dimensional photonic crystal cavities is far
behind due to the limitation in fabrication. This suggests that, considering current
*fabrication technologies, designs of high Q cavities that can be achieved even with *

small structural size, which can be practically fabricated, should be realized in order
*to demonstrate high Q cavities. *

This thesis aims to fill in the abovementioned gaps. Regarding to the two-
dimensional photonic crystal cavities, a cavity design based on simulations using
FDTD computational method, in which its principal parameter of design used to boost
*Q factor is fabrication-tolerant and can be precisely controlled, is to be realized. This *
is the first objective of this thesis. Another key objective of this thesis is to show how
*to achieve high Q cavities even there is no photonic bandgap. In order to do so, *
mechanisms of losses of light when the bandgap is absent and a way to suppress them
must be explicitly understood. In addition, experimental demonstrations should be
performed on the designed cavities to confirm the availability of the strong light
confinement in such counter-intuitive photonic crystal cavities. The last and most
*important objective is to demonstrate a high Q cavity in three-dimensional photonic *
crystals, which is one important step towards the acquisition of complete
manipulation of light-matter interaction, by means of proposing new designs of high
*Q cavities with finite structural size. The author’s original contributions to the field *
are briefly summarized in the following thesis outline.

**1.3 Thesis outline **

This thesis presents original research work on designs and fabrications of high
*Q nanocavities in both two- and three-dimensional photonic crystals. It is organized *
into eight chapters. Figure 1.1 shows how the eight chapters are logically related to
one another. Chapter 1 gives the research background and thesis objectives. It also
provides the reader with the thesis outline.

In Chapter 2, basic principles of photonic crystals are discussed to understand the behavior of light in photonic crystals and the origins of photonic band structures and bandgaps. Two-dimensional photonic crystal slabs with both triangular and square lattices and three-dimensional woodpile photonic crystal structures are then described in details as they are the basic building blocks of all the work in this thesis.

The influence of structural parameters, such as slab thickness and radius of air holes
of two-dimensional photonic crystal slabs, which are the important parameters of the
*designs of high Q nanocavities in Chapters 4 and 5, on the behavior of photonic *

bandgap is preliminarily discussed. Finally, photonic crystal nanocavities formed by introducing artificial defects into a perfectly periodic system are introduced.

Chapter 3 describes computational methods used in this thesis, which are all
based on the FDTD method. The FDTD simulations are categorized into two classes
with different boundary conditions. To calculate the fields in the infinitely extended
periodic system, i.e., to calculate photonic band diagram, periodic boundary condition
reduces the computational domain to a primitive cell of the crystal. In the case of a
finite structure, i.e., a photonic crystal structure with defect cavity, the entire structure
has to be set up in the core region of the simulation and perfectly matched layer is
exploited to enclose the region as a nonreflecting absorber, so that outgoing energy is
not reflected back to the core region. Then applications of the FDTD method, together
with the fast Fourier transformation, to the investigation of the characteristics of
*photonic crystal nanocavities, such as resonant frequencies, field distributions, Q *
factors, mode volumes of the cavity modes are presented.

**Figure 1.1 Thesis organization. **

Chapter 1 Introduction

Chapter 2 Basis for Theoretical Analysis of Photonic Crystal

Chapter 3 Finite-Difference Time-Domain Method

Chapter 4
*High-Q Photonic Crystal *
Nanocavity after Closing
of Photonic Bandgap
with Optimal Slab Thickness

Chapter 5
*High-Q Photonic Crystal *
Nanocavity without Photonic

Bandgap by Modulating Air Hole Radii in Square Lattice

Chapter 6
*Designs of High-Q*
Nanocavities in Three-Dimensional

Photonic Crystals with Finite Structural Sizes

Chapter 7

Fabrication and Characterization
*of High-Q Three-Dimensional *
Photonic Crystal Nanocavities

Chapter 8 Conclusions and Future Outlook

Chapter 1 Introduction

Chapter 2 Basis for Theoretical Analysis of Photonic Crystal

Chapter 2 Basis for Theoretical Analysis of Photonic Crystal

Chapter 3 Finite-Difference Time-Domain Method

Chapter 3 Finite-Difference Time-Domain Method

Chapter 4
*High-Q Photonic Crystal *
Nanocavity after Closing
of Photonic Bandgap
with Optimal Slab Thickness

Chapter 4
*High-Q Photonic Crystal *
Nanocavity after Closing
of Photonic Bandgap
with Optimal Slab Thickness

Chapter 5
*High-Q Photonic Crystal *
Nanocavity without Photonic

Bandgap by Modulating Air Hole Radii in Square Lattice

Chapter 5
*High-Q Photonic Crystal *
Nanocavity without Photonic

Bandgap by Modulating Air Hole Radii in Square Lattice

Chapter 6
*Designs of High-Q*
Nanocavities in Three-Dimensional

Photonic Crystals with Finite Structural Sizes

Chapter 6
*Designs of High-Q*
Nanocavities in Three-Dimensional

Photonic Crystals with Finite Structural Sizes

Chapter 7

Fabrication and Characterization
*of High-Q Three-Dimensional *
Photonic Crystal Nanocavities

Chapter 7

Fabrication and Characterization
*of High-Q Three-Dimensional *
Photonic Crystal Nanocavities

Chapter 8 Conclusions and Future Outlook

Chapter 8 Conclusions and Future Outlook

Chapters 4 and 5 concern work on the two-dimensional photonic crystal slab
nanocavities. Chapter 4 serves for the first thesis objective regarding to a proposal of
*achievement of high Q cavity by optimizing slab thickness. A significant increase of *
*Q factor of dipole modes in photonic crystal H1-defect nanocavity after closing of the *
photonic bandgap by tuning the slab thickness is numerically and experimentally
demonstrated. It is shown that the optimal slab thickness is equal to a wavelength of
light confined in the cavity, which is approximately two times thicker than that of
conventional structures. Interestingly, the strong light confinement of the cavity in the
in-plane direction is not caused by the photonic bandgap effect due to a lack of the
photonic bandgap but resulted from the decoupling between the cavity modes and the
guided modes in the momentum space yielding only weak coupling between these
two modes. This finding contributes to extending the freedom of cavity design. It is
also suggested that because the only parameter of this cavity that needs to be adjusted
is the slab thickness which can be precisely controlled by using epitaxial growth
techniques such as molecular beam epitaxy (MBE) or metal-organic chemical vapor
deposition (MOCVD), discrepancy of structural parameters between the designed and
the fabricated structures can be very small.

Chapter 5 deals with the second objective aiming to extend the scope of
*applications of high Q photonic crystal cavities to structures where a photonic *
bandgap does not exist. The concept of mode decoupling established in Chapter 4 is
*extended to design a cavity with higher Q and more flexible in applications by *
gradually modulating air hole radii in square lattice photonic crystals. An ultra-high
*ratio of Q factor to mode volume, desired for applications such as entangled photon *
source, of these modes has been achieved and this value is about two times higher
than the highest value reported so far. In addition, the designed cavity has been applied
*to achieve high Q cavities for material with low index and for quantum cascade lasers, in *
which a lack of photonic bandgap usually hinders them from applications. These
results emphasize a flexibility of the cavity, while the photonic bandgap is no longer a
*preliminary requirement to achieve high Q. *

The topic is then turned to discussions on three-dimensional structures. In
*Chapter 6, three designs of high Q cavities in three-dimensional photonic crystals *
with finite structural size that can be practically fabricated are presented. Two of them

to gain an advantage from the photonic bandgap effect as much as possible, and thus
*highest Qs, by means of optimizing size of the defect cavities. Apart from tuning *
*cavity modes to the midgap frequency, it is also theoretically predicted that the Q *
factor can be further increased more than four times in magnitude compared with that
of the unperturbed structure by slightly modifying the arrangement of dielectric rods
surrounding the cavity site.

In Chapter 7, the fabrication of the three-dimensional woodpile photonic
crystal nanocavities designed in Chapter 6 using micromanipulation techniques and
their optical characteristics are presented. Firstly, principles of the micromanipulation
techniques and how to use them to assemble three-dimensional structures are
described. The structures with a large number of stacked layers have been achieved
with high alignment accuracy. After that, experimental results are given on optical
characterization of the fabricated cavities coupled with quantum dots by means of
photoluminescence measurements. For the cavity with square-shaped in the 25-layer
*woodpile structure, a cavity mode with Q factor of more than 8,600, which is the *
*highest Q among those for three-dimensional photonic crystal cavities reported so far, *
has been achieved. This result is consistent with the calculation results discussed in
Chapter 6, in which a cavity mode locating closest to the midgap possesses the
*highest Q. Moreover, for a cavity with rectangular-shaped and smaller size, a cavity *
*mode with Q factor of more than 7,700 with an ultra-small mode volume of 2 cubic *
half-wavelengths has been obtained. The results presented in this chapter give three-
dimensional photonic crystals a wide-open opportunity for the realization of the
applications concerning the control of light-matter interaction.

Chapter 8 is the conclusion to this thesis. Implications of the results presented in this thesis are discussed. The outlook for future research and development is also given

**Chapter 2 **

**Basis for Theoretical Analysis of ** **Photonic Crystal **

Photonic crystal, which is a periodic arrangement of dielectric media, introduces a periodic potential to photons propagating through it in the same way as a crystal, in which electron experiences a periodic potential due to a periodicity of atoms or molecules, in electronic systems. This “optical potential” leads to the development of a band structure for photons in photonic crystals. Resulting photonic bandgaps which disallow the propagation of light in the crystal for frequencies inside the gap and artificially introduced defects can be applied to construct, for example, mirror, waveguide, or nanocavity structures. In order to accurately describe the behavior of light in photonic crystals, the full vector nature of light has to be taken into account using the Maxwell’s equations.

**2.1 Maxwell’s equations and the Bloch-Floquet theorem **

The macroscopic electromagnetic fields are described by the Maxwell’s equations

*t*

*H*
*E* *c*

∂

− ∂

=

×

∇ r r

r 1

(2.1)

*t*
*E*
*J* *c*

*H* *c*

∂ + ∂

=

×

∇

r r r

r 4π 1 ε

(2.2)
*∇ E*r⋅εr =4πρ

(2.3)
*∇ H*r⋅ r =0

(2.4)
where )*E r*r*( tr*,

and *H r*r*( tr*, )

* are the electric and magnetic fields, which can be *
expressed by:

*E*r(*r*r,*t*)=*E*r(*r*r)*e*^{i}^{ω}^{t}

(2.5)

*H*r(*r*r,*t*)=*H*r(*r*r)*e*^{i}^{ω}^{t}

(2.6)
*J*r

is the free current density, ρ is the free charge density, and ε is the dielectric
function. In the case that light propagating within a dielectric medium without any
light sources, *J*r

and ρ can be set to zero. In addition, it is acceptable to restrict the dielectric function ε to the case of linear dielectrics. And also, ε is assumed to be independent of frequency and being a real number.

According to these assumptions, by substituting Eq. (2.5) and Eq. (2.6) into Eq.

(2.1) and Eq. (2.2) and then combining them into one equation, which contains only )

*(r*
*H r*r

components, called the master equation:

( ) ( )

) (

1 ^{2}

*r*
*c* *H*
*r*

*r* *H*

r r r r

r r

r ⎟

⎠

⎜ ⎞

⎝

=⎛

⎟⎟⎠

⎜⎜ ⎞

⎝

⎛ ∇×

×

∇ ω

ε (2.7)
Then use Eq. (2.2) to regain*E(r*):

( )

) ) (

( *H* *r*

*r*
*r* *ic*

*E* r r r

r r

r ⎟⎟⎠∇×

⎜⎜ ⎞

⎝

=⎛ −

ωε (2.8)
It can be observed from Eq. (2.7) that it is a Hermitian eigenvalue problem an
eigenfunction )*H r*r*(r*

* and an eigenvalue (*ω*/c)*^{2}. The eigenfunctions *H r*r*(r*)

are the allowed fields in the structure, i.e., the electromagnetic modes of the system.

An important feature of the electromagnetic modes is that there is no
specified length scale involved. Once the eigenvalues and eigenfunctions of Eq. (2.7)
are solved, they can be scaled to any physical size or wavelength range. This can be
understood by defining*r*r =′ *sr*r,∇′r =∇r /*s*

, and ε′(*r*r)=ε(*r*r/*s*), and substituting them
into Eq. (2.7). This results in

) / ( )

/ ) (

/ (

1 ^{2}

*s*
*r*
*c* *H*
*s*

*r*
*H*
*s* *s*

*s* *r* r r r r r

r r

⎟⎠

⎜ ⎞

⎝

=⎛

⎟⎟⎠

⎜⎜ ⎞

⎝

⎛ ∇×

×

∇ ω

ε (2.9)

whereε(*r*r/*s*)=ε′(*r*r)*. Thus *

) / ( )

/ ) (

(

1 ^{2}

*s*
*r*
*cs* *H*
*s*

*r*
*r* *H*

r r r r

r r

r ⎟ ′

⎠

⎜ ⎞

⎝

=⎛

⎟⎟⎠

⎜⎜ ⎞

⎝

⎛ ∇′× ′

′

× ′

∇′ ω

ε (2.10)

*It can be seen that when the dimensions are scaled by a factor of s, the *
electromagnetic mode is the same, but has to be scaled as*H r*r(*r*/*s*)

and the frequency

designed without specifying the dimensions and subsequently fabricated in an scale to perform experiments in varying wavelength ranges.

Because a photonic crystal is a periodically ordering dielectric media, its
dielectric function ε*(rr*) becomes a periodic function of positions. The solution of the
Hermitian eigenvalue problem shown in Eq. (2.7) can always be shown in the form of

*r*
*k*

*e**i*^{r}^{⋅}^{r}(periodic function), where *k*r

is the wave vector. This is commonly known as Bloch-Floquet theorem [83]. A periodic function is expressed as:

*u*r_{k}_{r}(*r*r)=*u*r_{k}_{r}(*r*r+*R*r) (2.11)
for any lattice vector Rr

. If the function is periodic in all three dimensions, lattice
*vector R*r

can be formed in:

*R*r *la*r_{1} *ma*r_{2} *na*r_{3}
+
+

= (2.12)
*where (l, m, n) are integers and ar*_{1}, *ar*_{2} and *ar are primitive lattice vectors. *_{3}

Therefore, the solution of Eq. (2.7) for a periodic dielectric function ε is given by:

) ( )

( )

(*r* *e* *u* *r* *e* *u* *r* *R*

*H*r* _{k}* r

^{i}

^{k}*r*

^{r}*r*

_{k}

^{i}

^{k}*r*

^{r}*r r*

_{k}r r r r r

r

r = ^{⋅} = ^{⋅} + (2.13)
This Bloch state indicates each electromagnetic mode through its wave vector *k*r

and
periodic function*u*r_{k}_{r}*(r*r). To solve for*u*r_{k}_{r}*(r*r), Eq. (2.13) is substituted into Eq. (2.7),
another Hermitian eigenvalue problem is then obtained:

1( ) ( ) ( )

) (

2

*r*
*c* *u*

*r*
*u*
*k*
*i*
*k*

*i*r r r r* _{k}* r r

*r*

_{k}r r ⎟ r

⎠

⎜ ⎞

⎝

=⎛

× +

∇

× +

∇ ω

ε (2.14)
Due to the periodicity of*u*r_{k}_{r}*(r*r), Eq. (2.14) can be considered as the eigenvalue
problem over a unit cell of the photonic crystal. Corresponding to quantum mechanics,
eigenvalue problem with a finite domain leads to a discrete set of eigenvalues. That is,
there is a set of modes, denoted by _{n}*(k*r)

ω (for band number n = 1, 2, 3, …), which are
discretely spaced in frequencies and continuously varied as *k*r

varies. The plot of
these frequency bands as a function of *k*r

is called the band structure of photonic crystal.

Another important property of the Bloch states is that, in order to solve the
eigenvalue problem for a wavevector*k*r

, it is adequate to only solve the eigenvalue
problem for *k*r

in a finite zone called the first Brillouin zone. By considering the
Bloch state shown in Eq. (2.10), an eigensolution with wave vector *k*r

is identical to

an eigensolution with wave vector*k*r *G*r

+ , where *G*r

is a reciprocal lattice vector and defined as:

3 2

1 *mb* *nb*

*b*
*l*

*G*r r r r

+ +

= (2.15)
*where (l, m, n) are integers and b*r_{1}

, *b*r_{2}

and *b*r_{3}

are primitive reciprocal lattice vectors.

This vector can be evaluated from *G*r⋅*R*r= *N*2π

*(for N = 1, 2, 3, …). This means that, *
in order to solve the eigenvalue problem for*k*r

, *k*r

will be bounded to only the region
in reciprocal space where *k*r

cannot have any other values of itself by adding any*G*r
.
This restricted region is called the first Brillouin zone. Furthermore, if additional
symmetries, e.g., rotational symmetry, are applied to photonic crystals, it is
**unnecessary to solve for every ***k*r

point in the first Brillouin zone. Only the region, in
which those symmetries do not have any effects on ω_{n}*(k*r), is required. This region is
called the irreducible Brillouin zone.

**2.2 Origin of photonic bandgap **

In certain structures of photonic crystal there can be a range of ω, in which no
propagating states ω_{n}*(k*r) corresponding to the restricted wave vector *k*r

are allowed and all incident radiation is reflected. This frequency range is known as the photonic band gap. In order to understand the origin of the gap, two properties of Hermitian eigenvalue problem have to be concerned. Firstly, because the operator of Eq. (2.7) is Hermitian, its eigenvalue must be real and positive and its harmonic modes must be orthogonal:

*H*r_{1} *H*r_{2} =0

(2.16) That is, an inner product of any two harmonic modes with different frequencies is zero. Secondly, corresponding to the electromagnetic variational theorem, the lowest frequency mode is the field pattern that minimizes the electromagnetic energy functional:

2 1 2

) , ( 2

1 1

) , ( 2 ) 1

( *E*

*r* *c*
*H* *d*
*H* *H*

*r*
*H* *d*
*H* *H*

*E** _{f}* r r r r r r r r r ωε r

ε

ε

### ∫

### ∫

⎟⎟⎠

⎜⎜ ⎞

⎝

=⎛

×

⎟⎟ ∇

⎠

⎜⎜ ⎞

⎝

=⎛ (2.17)

Other higher bands, e.g., the second band, also satisfy Eq. (2.17), but orthogonality of

the regions of high dielectric constant ε to lower its potential energy. This yields to
have a lower frequency. Additionally, the curl of field *H*r

×

∇ should be small, in
other words, the field is varying slowly inside the high dielectric constant regions and
containing no nodal plane, in order to lower its kinetic energy. When the case comes
to the second band, this mode also wants to be concentrated in the high dielectric
constant regions and contain no nodal plane inside those regions to obtain the
*minimum E**f*. However, from Eq. (2.16), this mode must be orthogonal to the mode of
the first band. As a result, the second band has to be concentrated in the regions of
low dielectric constant and restrictedly have nodal plane in those regions to make the
integral zero. This results in a difference in frequencies of these two bands and the
band gap occurs. This can be understood by an example shown in Fig. 2.1(a).

*Applying the relation in Eq. (2.17), two equally symmetric modes, sin(πx/a) and *
*cos(πx/a), are forced in a one-dimensional photonic crystal. The bandgap between the *
top of dielectric band and bottom of air band is visualized for a one-dimensional
photonic crystal in Fig. 2.1(b).

Unlike the simple one-dimensional photonic crystal, in which any nonzero periodic dielectric variation will result in a complete bandgap, achieving a photonic bandgap in higher-dimensional photonic crystal becomes complicated. This is because the forbidden gaps for all possible directions in reciprocal space are needed to be overlapped in some frequency. Therefore, with a fairly large contrast in ε between the high and low dielectric regions, a proper geometry of the periodic structure should be selected to create the photonic bandgap. Figure 2.2(a) shows the Brillouin zone of the face-centered-cubic lattice. A point on the surface of the Brillouin zone closest to the center is the L point, oriented toward the body diagonal of the cube. A point in the cubic direction is the X point. Considering a plane wave in the X direction as done in the case of the one-dimensional photonic crystal, it will sense the periodicity in the cubic direction, forming a standing wave and opening a forbidden gap as indicated by the shading in Fig. 2.2(b). Supposing, on the other hand, that the plane wave is going in the L direction, it will sense the periodicity along the cubic-body diagonal, and a gap will form in that direction as well. But the wave vector to the L point is ~ 14%

smaller that the wavevector to the X point. Therefore, the gap at L is likely to be centered at a 14% smaller frequency than the gap at X. If the two gaps are not

**Figure 2.1 (a) Schematic illustration of the electric fields of mode at air and **
*dielectric bandedges in a multilayer film with lattice constant a. (b) Photonic band *

**a**

**a**

**sin(πx/a)**

**cos(πx/a)**

**Low-**ε **High-**ε

**-0.5 -0.25 0 0.25 0.5 **
**0.00**

**0.05**
**0.10**
**0.15**
**0.20**
**0.25**
**0.30**

### Photonic bandgap

**Wave vector (ka/2π)**

**Wave vector (ka/2π)**

**F** **requen** **cy (** **a/** **λ)**

**a/**

**a**

**a**

**sin(πx/a)**

**cos(πx/a)**

**Low-**ε **High-**ε

**a**

**a**

**sin(πx/a)**

**cos(πx/a)**

**Low-**ε **High-**ε

**-0.5 -0.25 0 0.25 0.5 **
**0.00**

**0.05**
**0.10**
**0.15**
**0.20**
**0.25**
**0.30**

### Photonic bandgap

**Wave vector (ka/2π)**

**Wave vector (ka/2π)**

**F** **requen** **cy (** **a/** **λ)**

**a/**

**(a) **

**(b) **

wide enough, they will not overlap in frequency. As a result, for three-dimensional photonic crystal, the Brillouin zone should most closely resemble a sphere in order to increase the likely hood of a frequency overlap in all directions of space. In this case, the face-centered-cubic lattice has the highest potential among any other types of lattice to achieve a photonic bandgap due to its least percentage deviation of the Brillouin zone from a sphere.

In the same way as in the three-dimensional system, the two-dimensional photonic crystals whose the Brillouin zone more closely resemble a circle will lead to a larger gap. This will be discussed in details in next subsection.

**2.3 Types of photonic crystals **

According to the order of dimensions that they periodically alter, photonic crystals can be classified into three categories, which are one-dimensional, two- dimensional, and three-dimensional photonic crystals. These three types of photonic crystal are shown in Fig. 2.3. In one- and two-dimensional photonic crystals,

**Figure 2.2 (a) Brillouin zone of face-centered-cubic lattice. (b) Forbidden gap **
(shaded) at point L, which is centered at a frequency ~ 14% lower than X-point
forbidden gap.

**(a) (b) **

**Frequen** **cy (** **a/** **λ)**

**a/**

**k** **L X**

**Frequen** **cy (** **a/** **λ)**

**a/**

**k** **L X**

**Frequen** **cy (** **a/** **λ)**

**a/**

**k**

**L X**

band structure diagrams and bandgaps are limited to the directions of periodic dielectric modulation. Unaffected propagation of electromagnetic waves is possible along those lattice directions showing no periodicity [84]. One-dimensional photonic crystals are known as Bragg mirrors. These structures have been used for a long time before the concept of photonic crystals was established, but the same concepts and principle apply to the one-dimensional structures also. They consist of periodically stacked layers of different refractive indices [85]. Two-dimensional photonic crystals have a periodicity in two dimensions and are infinitely extended in the third dimensions. They are often realized in practice by a periodic arrangement of air cylinders in a dielectric or by cylinders consisting of a dielectric material in air organized in a square or triangular lattice. [86-89]. Three-dimensional photonic crystals are the only true photonic crystals in the strict sense since in them light propagation can be forbidden in all directions. In the following subsections, only two- dimensional photonic crystal slabs with both triangular and square lattices and three- dimensional (woodpile) photonic crystal structures will be discussed as they are the basic building blocks of the work described in this thesis.

**2.4 Two-dimensional photonic crystal slabs **

**Figure 2.3 Schematic illustrations of photonic crystal (a) one-dimensional (b) two-**
dimensional (c) three-dimensional.

**(a) ** **(b) ** **(c) **

infinite structures in the third dimension. Therefore, the concept of a two-dimensional photonic crystal slab was proposed to overcome this obstacle [57]. Two-dimensional photonic crystal slab is essentially a two-dimensional photonic crystal with a finite third dimension. One typical structure is a membrane based photonic crystal shown in Fig. 2.4. An optically thin semiconductor slab (thickness is roughly λ/2) is surrounded with a low-refractive index material (usually air), and perforated with a two- dimensional lattice of holes. When the slab is cladded by air on both sides, the structure is called a two-dimensional air-bridge photonic crystal. In such structure, the localization of light in all three dimensions is made possible by the combination of two mechanisms: in the vertical direction, light is confined to the slab by means of total internal reflection due to high index contrast between the high-index slab and the low-index environment, while in the in-plane direction light is controlled by means of distributed Bragg reflection due to the presence of two-dimensional lattice of holes. In the two-dimensional air-bridge photonic crystal shown in Fig. 2.4 the third dimension is not periodic nor infinite, and therefore photons incident to the surface between the semiconductor slab and air with smaller angles than the critical angle for total internal reflection can escape from the slab and couple into the continuum of radiation modes.

These photons leak energy from the slab and therefore represent the loss mechanism of the two-dimensional photonic crystal slab. In order to take these losses into account, the notion of light cone is introduced in the analysis of photonic crystal by the light line. The light cone, where the leaky modes exist, is the region over the light line.

**Dielectric **
**slab **
**Air **

**Air **

**Active ** **Air **

**Figure 2.4 Schematic illustration of photonic crystal slab. **

The light cone, where the leaky modes exist, is the region over the light line.

Concretely, examining the energy-momentum dispersion relation for a homogeneous
*dielectric cladding with refractive index n: *

^{2} ^{2}

2

⊥

∠ +

⎟ =

⎠

⎜ ⎞

⎝

⎛ *k* *k*

*c*
*n*ω

(2.18)
where ω is the angular frequency, *k*_{∠}is the in-plane wave vector, *k*_{⊥}is the wave
*vector normal to the slab, and c is the speed of light. Light line can be confined as: *

2

2 ⎟

⎠

⎜ ⎞

⎝

=⎛

∠ *c*

*k* *n*ω

(2.19) Since radiative modes exist at all frequencies, including the bandgap region, they close the bandgap, and the complete bandgap does not exist in two-dimensional photonic crystal slab. The forbidden frequency range still exists, however, for the guided modes of the slab, which is for the photons confined in the patterned slab and just decayed exponentially into the claddings. The gap for guided modes is shown by shaded region in Fig. 2.5. Therefore, in the case of two-dimensional photonic crystal slab, the bandgap is not complete and it exists only for the guided modes of the patterned slab. The properties of two-dimensional photonic crystal slab, such as position and width of the bandgap, depend strongly on several important parameters:

the type of lattice (e.g., triangular, square), the thickness of the slab (d), the refractive of both slab and claddings, the periodicity of the lattice (a) and the radius of the holes (r).

In two-dimensional photonic crystal, due to the mirror reflection symmetry in the direction perpendicular to the plane of periodicity, modes of every two- dimensional photonic crystal can be classified into two non-interacting classes of polarizations: TE polarized modes (electric field in plane of periodicity) and TM polarized modes (magnetic field in plane of periodicity). As in two-dimensional system, guided modes in photonic crystal slab can be also decomposed into two distinct classes. These are not purely TE and TM polarized as in the two-dimensional photonic crystal due to the finite extent of slab in the direction normal to the plane of slab. However, they are classified by whether they transform to be even or odd with respect to a horizontal mirror plane bisecting the slab. These even and odd states have the strong similarities with TE and TM modes, respectively, in two-dimensional

photonic crystal. In addition, within the slab they are TE- and TM-like, and closely resemble the TE and TM modes in two-dimensional system.

**2.4.1 Comparison between square and triangular photonic crystal lattices **
Since in this thesis, two-dimensional photonic crystal slabs with two types of
lattice, square and triangular, are concerned, they will be discussed in details in this
subsection. The structure that is a GaAs slab, suspended in air, and patterned with
square or triangular lattice of holes as illustrated in Fig. 2.6 and 2.7. The Three-
dimensional Finite-Difference Time-Domain method (3D-FDTD) was used to
calculate the band diagrams (details on the computational method are discussed in
Chapter 3). The thickness of the slab was d = 0.60a and hole radius was r = 0.40a.

The refractive index of GaAs is assumed to be 3.4.

**Figure 2.5 Band diagram for the air-bridge slab structure with r = 0.30a and d = **
0.60a. The insets show triangular lattice of air holes in dielectric with refractive
index of 3.4 and its first Brillouin zone.

**Figure 2.7 The triangular lattice shown in (a) real space and (b) reciprocal space **
with their corresponding lattice vectors. The hexagon represents the first Brillouin
zone, and Γ, K and M are the high-symmetry points.

**y **

**x **

**k****y**

**k****x**

**a****a****1 **

**a****2 **

**(2π/a) **
**b****1**

**b****2**

**X **
**M **
Γ

**(a) (b) **

**y **

**x ** **a **

**a****2 **

**a****1 **

**k****y**

**k****x**

**b****2**

**b****1**

**M **
Γ **K **

**(a) (b) **
**Figure 2.6 The square lattice shown in (a) real space and (b) reciprocal space with **

their corresponding lattice vectors. The square represents the first Brillouin zone, and Γ, X and M are the high-symmetry points.

Figure 2.6 (a) and (b) illustrate the square lattice in real space and reciprocal space, respectively. The lattice vectors in real space are

) 0 , 0 , 1

1 *= a*⋅(

*ar* and*ar*_{2} *= a*⋅(0,1,0), and reciprocal lattice vectors are*b*^{r}_{1} =(2π/*a*)⋅(1,0,0)
and*b*^{r}_{2} =(2π/*a*)⋅(0,1,0). The square in Fig. 2.6(b) represents the first Brillouin zone,
and Γ, X and M are the high-symmetry points with coordinates in reciprocal space: Γ

= (0,0,0), X = (π/a,0,0), M = (π/a,π/a,0). In the case of the photonic crystal slab with
triangular lattice, lattice vectors in the real space can be expresses
as*ar*_{1} *= a*⋅(1/2, 3/2,0)and*ar*_{2} *= a*⋅(1/2,− 3/2,0), and reciprocal lattice vectors are

) 0 , 2 / 1 , 2 / 3 ( ) / 2

1 =( *a* ⋅

*b*^{r} π and*b*^{r}_{2} =(2π/*a*)⋅( 3/2,−1/2,0) . The hexagon in Fig.

2.7(b) represents the first Brillouin zone, and the coordinates of high-symmetry points
are Γ= (0,0,0), *M* =(π/*a*)⋅(1,1/ 3,0), *K* =(π/*a*)⋅(4/3,0,0).

Band diagram for the vertically even (TE-like) eigenmodes of the two- dimensional photonic crystal slab structure with square and triangular symmetry are shown in Fig. 2.8. Only band diagram for TE-like modes are concerned here since active materials adopted in this work are quantum dots, which have electronic states predominantly coupled to the TE modes. As it can be seen, in both structures the first- order bandgap is open for the guided modes of the slab. The bandgap is formed only for the guided modes as discussed above. The photonic crystal slab with triangular lattice has a much wider bandgap than the square lattice, a result of the greater symmetry and the smoother Brillouin zone in that geometry, in other words, the Brillouin zone more closely resemble a circular shape. Therefore, the triangular lattice is in many ways a more promising geometry for the realization of photonic crystal devices. However, in many cases it is not necessary to work with photonic crystals that have wide bandgap. In Chapter 4 and 5, it will be shown that high quality factor cavity can be realized in the structures with a very small bandgap or even no bandgap at all.

**2.4.2 Effect of slab thickness and radius of air holes on photonic bandgap **

Because high quality factor photonic crystal nanocavities by optimizing the slab thickness and by modulating air hole radii will be presented in Chapter 4 and 5, respectively, in this subsection the influence that slab thickness and radius of air holes have on the behavior of photonic bandgap is discussed. A triangular lattice